   MI: Initial Torque
This calculation returns the Maximum Torque recorded at Test Start.

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: dN*m or Lbf*In

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S') ML: Minimum Torque
This calculation returns the minimum torque value measured during the test;

The calculation provides useful information regarding the viscosity of the green compound at test temperature.
For example, this information may be useful for:
- the correct evaluation of the force needed for injection moulding (depending from the shape of the mould and the size of the injection channels)
- the setting of temperature and force for extrusion process.

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: dN*m or Lbf*In

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S') tML: Time at Minimum Torque
This calculation returns the time, from the start of the test, when the ML point is reached (in the case of maintenance of the ML value over a period of time, it represents the termination point of the interval)

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S')  MH: Maximum Torque
This calculation returns the maximum torque value measured during the established test time.

Depending from the product under test, from the test time selected and from the test temperature, the curve may have reached a plateau value or not
This calculation is an indication of the mechanical characteristics of the cured compound and has positive correlation with other mechanical properties like hardness and tensile stress at set strain.

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: dN*m or Lbf*In

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S') tMH: Time at Maximum Torque
This calculation returns the time, from the start of the test, when the MH point is reached (in the case of maintenance of the MH value over a period of time, it represents the starting point of the interval)

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S') ts_x: Scorch Time
The Scorch time tsx is the time required for the torque to increase by x units from ML. The typical value of x for an MD Rheometer is 1 dN•m.

The scorch time (time to incipient cure) tsx is a measure of the processing safety of the compound.
For injection moulding, it provides a relative indication of the maximum available time for the complete filling of the cavities.

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S')  t'_x: time to set percentage of curing
The time to a percentage of full cure from minimum torque t’_x is the time taken for the torque to reach: ML + x*(MH-ML)/100
Frequently used values of t’_x are:
- t’_10: is a measure of the early stages of cure
- t’_50: provides the slope of the curve is greatest at this point.
- t’_90: is often used as an indicator of optimum press cure

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

CALCULATION PARAMETERS:
Percentage of Curing desired.
Reference Curve (0=S*,1=S') M_x: torque at set percentage of curing
Torque at a percentage of full cure from minimum torque M_x is the torque value at: ML + x*(MH-ML)/100

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: dN*m or Lbf*In

CALCULATION PARAMETERS:
Percentage of Curing desired.
Reference Curve (0=S*,1=S') Tanƌ@ML: Tangent of ƌ at Minimum Torque
This calculation returns the reading of the Tanƌ curve when S' curve reaches ML.
The calculation is an expression of visco-elastic properties of the uncured sample.

UNIT: num  Tanƌ@MH: Tangent of ƌ at Maximum Torque
This calculation returns the reading of the Tanƌ curve when S' curve reaches MH.
The calculation is an expression of visco-elastic properties of the cured sample.

UNIT: num S"@ML: Viscous curve at Minimum Torque
This calculation returns the reading of the S" curve when S' curve reaches ML.
The calculation is an expression of viscous properties of the uncured sample.

UNIT: dN*m or Lbf*In S"@MH: Viscous curve at Maximum Torque
This calculation returns the reading of the S" curve when S' curve reaches MH.
The calculation is an expression of viscous properties of the cured sample.

UNIT: dN*m or Lbf*In  tR_x: Time for Reversion of x dN*m
This calculation returns the time from test start, when a torque reduction of x dN*m from MH is detected.
The calculation is an expression of the degradation of the sample at the testing conditions.

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

CALCULATION PARAMETERS:
Torque decay compared to MH
Reference Curve (0=S*,1=S') Rev_t: Reversion at set Time
This calculation returns the torque reduction from MH at the set test time.
The calculation is an expression of the degradation of the sample at the testing conditions.

UNIT: dN*m or Lbf*In

CALCULATION PARAMETERS:
Test time
Reference Curve (0=S*,1=S') MCR: Maximum Curing Rate
This calculation returns the maximum torque increase value in the time unit measured during the test (corresponds to flexure point of the increasing line of the elastic curve S')

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: dN*m/sec  TMCR: Time at Maximum Curing Rate
This calculation returns the time from test start at Maximum Cure Rate

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds  Gibitre Instruments
Via dell'industria, 18
Bergamo (Italy)
te. +39 035 461146
www.gibitre.it
info@gibitre.it

� Gibitre Instruments # RheoCheck: Test Results

## Below you can find the description of the test results produced by RheoCheck software MI: Initial Torque
This calculation returns the Maximum Torque recorded at Test Start.

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: dN*m or Lbf*In

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S')

ML: Minimum Torque
This calculation returns the minimum torque value measured during the test;

The calculation provides useful information regarding the viscosity of the green compound at test temperature.
For example, this information may be useful for:
- the correct evaluation of the force needed for injection moulding (depending from the shape of the mould and the size of the injection channels)
- the setting of temperature and force for extrusion process.

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: dN*m or Lbf*In

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S')

tML: Time at Minimum Torque
This calculation returns the time, from the start of the test, when the ML point is reached (in the case of maintenance of the ML value over a period of time, it represents the termination point of the interval)

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S')

MH: Maximum Torque
This calculation returns the maximum torque value measured during the established test time.

Depending from the product under test, from the test time selected and from the test temperature, the curve may have reached a plateau value or not
This calculation is an indication of the mechanical characteristics of the cured compound and has positive correlation with other mechanical properties like hardness and tensile stress at set strain.

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: dN*m or Lbf*In

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S')

tMH: Time at Maximum Torque
This calculation returns the time, from the start of the test, when the MH point is reached (in the case of maintenance of the MH value over a period of time, it represents the starting point of the interval)

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S')

ts_x: Scorch Time
The Scorch time tsx is the time required for the torque to increase by x units from ML. The typical value of x for an MD Rheometer is 1 dN•m.

The scorch time (time to incipient cure) tsx is a measure of the processing safety of the compound.
For injection moulding, it provides a relative indication of the maximum available time for the complete filling of the cavities.

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

CALCULATION PARAMETERS:
Reference Curve (0=S*,1=S')

t'_x: time to set percentage of curing
The time to a percentage of full cure from minimum torque t’_x is the time taken for the torque to reach: ML + x*(MH-ML)/100
Frequently used values of t’_x are:
- t’_10: is a measure of the early stages of cure
- t’_50: provides the slope of the curve is greatest at this point.
- t’_90: is often used as an indicator of optimum press cure

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

CALCULATION PARAMETERS:
Percentage of Curing desired.
Reference Curve (0=S*,1=S')

M_x: torque at set percentage of curing
Torque at a percentage of full cure from minimum torque M_x is the torque value at: ML + x*(MH-ML)/100

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: dN*m or Lbf*In

CALCULATION PARAMETERS:
Percentage of Curing desired.
Reference Curve (0=S*,1=S')

Tanƌ@ML: Tangent of ƌ at Minimum Torque
This calculation returns the reading of the Tanƌ curve when S' curve reaches ML.
The calculation is an expression of visco-elastic properties of the uncured sample.

UNIT: num

Tanƌ@MH: Tangent of ƌ at Maximum Torque
This calculation returns the reading of the Tanƌ curve when S' curve reaches MH.
The calculation is an expression of visco-elastic properties of the cured sample.

UNIT: num

S"@ML: Viscous curve at Minimum Torque
This calculation returns the reading of the S" curve when S' curve reaches ML.
The calculation is an expression of viscous properties of the uncured sample.

UNIT: dN*m or Lbf*In

S"@MH: Viscous curve at Maximum Torque
This calculation returns the reading of the S" curve when S' curve reaches MH.
The calculation is an expression of viscous properties of the cured sample.

UNIT: dN*m or Lbf*In

tR_x: Time for Reversion of x dN*m
This calculation returns the time from test start, when a torque reduction of x dN*m from MH is detected.
The calculation is an expression of the degradation of the sample at the testing conditions.

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

CALCULATION PARAMETERS:
Torque decay compared to MH
Reference Curve (0=S*,1=S')

Rev_t: Reversion at set Time
This calculation returns the torque reduction from MH at the set test time.
The calculation is an expression of the degradation of the sample at the testing conditions.

UNIT: dN*m or Lbf*In

CALCULATION PARAMETERS:
Test time
Reference Curve (0=S*,1=S')

MCR: Maximum Curing Rate
This calculation returns the maximum torque increase value in the time unit measured during the test (corresponds to flexure point of the increasing line of the elastic curve S')

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: dN*m/sec

TMCR: Time at Maximum Curing Rate
This calculation returns the time from test start at Maximum Cure Rate

REFERENCE STANDARD: ISO 6502-1, ISO 6502-3

UNIT: mm:cc (minutes, minutes/100) or mm:ss (minutes, seconds) or Seconds

Related pages

Mail

Mail
Phone

Phone
Local agent

Local agent
FAQ
use the buttons at the bottom of the page.
Questo sito utilizza i cookies (dati permanenti registrati sul tuo PC) per:
- ricordare la lingua scelta
- ricordare i prodotti preferiti
- suggerire prodotti in funzione delle pagine più visitate
- mantenere aperta la sessione (nella sole aree riservata)

Cliccando su "accetta" autorizzate l'uso dei cookies.

Accetto / Accept